Loading in 2 Seconds...
Loading in 2 Seconds...
Diamond tip (5 m radius). Ferrule (2.5mm diameter). N ATIONAL S CIENCE F OUNDATION. Micro-Laser Assisted Machining (µ-LAM): Scratch Tests on 4H-SiC. Huseyin Bogac Poyraz, Amir R. Shayan, Deepak Ravindra, Muralidhar Ghantasala and John A. Patten (WMU, Kalamazoo, MI 49008 )
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
(5 m radius)
NATIONAL SCIENCE FOUNDATION
Micro-Laser Assisted Machining (µ-LAM): Scratch Tests on 4H-SiC
Huseyin Bogac Poyraz, Amir R. Shayan, Deepak Ravindra, Muralidhar Ghantasala and John A. Patten (WMU, Kalamazoo, MI 49008 )
2009 NSF CMMI Engineering Research and Innovation Conference, Honolulu, Hawaii
The objective of the current study is to determine the effect of temperature and pressure in the µ-LAM of the single crystal 4H-SiC semiconductors using scratch tests. The scratch tests examine the effect of temperature in thermal softening of the high pressure phases formed under the diamond tip. The tests also evaluate the difference with and without irradiation of the laser beam at a constant loading and cutting speed. The laser heating effect is verified by atomic force microscopy (AFM).
90° Conical diamond tip with 5 μm radius
FIGURE 2. 5 µm radIus dIamond tIp attached on the end of the ferrule usIng epoxy.
FIGURE 3. Close up on diamond tip embedded in the solidified epoxy.
FIGURE 1. A SCHEMATIC CROSS SECTION OF THE µ-LAM PROCESS.
FIGURE 4. µ-LAM system used in experiments.
The laser emerges from a 90 conical single crystal diamond tip with 5μm radius spherical end, as shown in Figure 2 and 3.
The µ-LAM experimental setup is shown in Figure 4. The equipment used to carry out the scratch tests was the Universal Micro-Tribometer (UMT) from the Center for Tribology Research Inc. (CETR). This equipment was developed to perform comprehensive micro-mechanical tests of coatings and materials at the micro scale. This precise equipment allows for cutting speeds as low as 1µm/sec at nanometric cutting depths.
The IR diode laser used in this investigation is a Furukawa 1480nm 400mW IR fiber laser with a Gaussian profile and beam diameter of 10μm. The IR laser beam is guided from the diode laser through a 10µm fiber optic cable to the ferrule, which is attached to the diamond stylus. In this setup, the IR laser beam passes through the diamond tip (tool) and impinges on the SiC work piece material.
TABLE 1. specifications of the scratches.
FIGURE 5. AFM IMAGES OF THE SCRATCH #3
(No laser heating, 25mN load, 1µm/sec Scratching Speed).
*Experiments performed previously (Dong and Patten, 2005), **350 mW is the laser power, approximately 150 mW is actually delivered to the work piece material, the balance of the laser power is lost due to scattering and reflections (Dong, 2006).
FIGURE 7. AVERAGE GROOVE DEPTH MEASURED WITH AFM IN (nm) WITH TWO DIFFERENT SPEEDS AND W/ AND W/O LASER.
In this experiment, two scratches have been employed; with and without laser heating. The results obtained from these tests are then compared to previously obtained results (Dong and Patten, 2005). The load used for the scratch tests is 2.5g (~25mN) with a cutting speed of 1µm/sec. Previously performed scratch tests with cutting speeds of 305µm/sec are reported here for comparison to the present work (Dong and Patten, 2005). Table 1 summarizes the experimental conditions.
FIGURE 6. AFM IMAGE OF THE SCRATCH #4
(w/ laser heating, 25mN load, 1µm/sec Scratching Speed).
In the previous set of scratches performed at 305µm/sec, the difference in the depth of cut for w/ and w/o laser heating was measureable but not significant, indicating some but not much laser heating and thermal softening. In the current set of scratches with 1µm/sec cutting speed, the depth of cut significantly increases with laser heating, nearly doubling, from 54 (w/o laser heating) to 90nm (see Figure 7). This latter result indicates significant laser heating and resultant thermal softening occurred. This result shows that temperature plays a significant role in enhancing the ductile regime machining of 4H-SiC specimen at this speed.
AFM measurements, shown in Figures 5 and 6, have been used to measure the groove size and to study the laser heating effect of the scratches made on 4H-SiC.
Laser heating was successfully demonstrated as evidenced by the significant increase in groove depth, i.e., reduced hardness, indicative of enhanced thermal softening. AFM measurements of the laser-heat assisted scratch grooves show deeper and wider grooves compared to scratches made without the laser heating assisted methods; which indicates favorable thermal softening effects.
The authors would like to thank NSF for funding this project by a grant from NSF CMMI-0757339. The authors would also like to thank Dr. Valery Bliznyuk and James Atkinson from Paper Engineering, Chemical Engineering and Imaging (PCI) Department of the Western Michigan University for providing the AFM results and Cree Inc. for providing 4H-SiC wafers.